Author's Accepted Manuscript
Dry sliding wear behaviour of AlSi-CNTs-SiCp Hybrid composites O. Carvalho, M. Buciumeanu, S. Madeira, D. Soares, F.S. Silva, G. Miranda
PII: DOI: Reference:
S0301-679X(15)00182-6 http://dx.doi.org/10.1016/j.triboint.2015.04.031 JTRI3658
To appear in:
Received date: 14 December 2014 Revised date: 16 April 2015 Accepted date: 19 April 2015 Cite this article as: O. Carvalho, M. Buciumeanu, S. Madeira, D. Soares, F.S. Silva , G. Miranda, Dry sliding wear behaviour of AlSi-CNTs-SiCp Hybrid composites, Tribology International, http://dx.doi.org/10.1016/j.triboint.2015.04.031 This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customers we are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, and review of the resulting galley proof before it is published in its final citable form. Please note that during the production process errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.
Dry sliding wear behaviour of AlSi-CNTs-SiCp hybrid composites O. Carvalhoa, M. Buciumeanub*, S. Madeiraa, D. Soaresa, F. S. Silvaa, G. Mirandaa a
CT2M – Centre for Mechanical and Materials Technologies, University of Minho, Azurem, 4800-058 Guimaraes, Portugal b Cross–Border Faculty of Humanities, Economics and Engineering, “Dunărea de Jos” University of GalaĠi, Domnească 47, 800008 Galati, Romania Emails: [email protected]
, [email protected]
, [email protected]
, [email protected]
, [email protected]
, *Corresponding author: Mihaela Buciumeanu, email: [email protected]
; Tel.: +351917560788; Fax.: +351253516007
Abstract The aim of this paper was to examine the wear behaviour of a hybrid AlSi-2wt. %CNTs5wt.%SiCp composite. For comparison purposes the unreinforced AlSi alloy, AlSi-2%wt.CNTs and AlSi-5wt.%SiCp composites were used. A powder metallurgy processing route was used to produce the unreinforced AlSi alloy and AlSi composites. Dry reciprocating pin-on-plate wear tests were performed and the results showed that the wear behaviour was improved for all produced composites when compared to the unreinforced AlSi alloy. However the best wear behaviour was achieved in the case of AlSi hybrid composite. This improvement is attributed to the combine effects of both constituent reinforcements. The dominant wear mechanisms were characterized by scanning electron microscopy with X-Ray Energy Dispersive Spectrometry analysis. Keywords: CNTs; AlSi- hybrid composites; SiCp; sliding wear.
1. Introduction It is well known that the specific strength of the materials used in the aerospace, aircraft and automotive industries is a key factor [1,2]. Besides, these materials should exhibit a good compromise between mechanical, physical and tribological properties. For example, in practice the piston rings damage is attributed first to wear, then to lubrication and fatigue . Aluminumsilicon (AlSi) alloy is a good choice for engine components [1,3], due to their satisfactory mechanical and wear properties. The reinforcements incorporated in the Al alloys are used to increase desired properties, which make them attractive for specific applications. Some of reinforcements used in the case of Al alloys are SiCp [4-6], Al2O3 , TiC , TiAl , B4C , TiB2 , CNTs [12-15], graphite , etc. Regarding the processing route, it is well known that by powder metallurgy (PM) it is possible to obtain a very good distribution of the particles. It should me also mentioned that the hot pressing allows a good densification process . Regarding aluminium (Al) alloy reinforced by carbon nanotubes (CNTs), and to the authors’ knowledge, there are only few studies [12-15,17-20] that are concerned with their wear behaviour. Most of the previous studies demonstrated that the CNTs are an effective reinforcement for improving wear characteristics of Al based composites [12-15]. The wear behaviour is explained based on CNT dispersion, CNT agglomeration size and fraction and carbide formation . Regarding the coefficient of friction (COF) as reported by other studies [12-15,17-20] it decreases with CNTs content, possibly due to the self lubrication effect of carbon content. Also, it was observed a reduction on COF when the agglomerations are formed (improving the wear resistance), as they act as a lubricant between the contacting surfaces . It has been reported that there is a critical CNTs agglomeration concentration, above which starts the well known detrimental effect. Regarding the effect of CNTs content (from 2 wt.% to 6 wt.% CNTs) over the mechanical and wear behaviour of AlSi-CNTs composites, it was concluded on a previous research work of the same authors [21,22] ,that in the case 2wt.%CNTs content there is an equilibrium among improvement in mechanical properties in the different tests namely tensile, fatigue and wear. It was concluded that the 2wt.%CNTs was the optimal CNTs content for tensile properties. Thus, in order to improve wear properties without reducing tensile values, another reinforcement, that would introduce a different strengthening mechanism or the some strengthening mechanism, but at a different scale, would be necessary. SiCp as a second reinforcement, was used in the present work. SiCp as reinforcement of Al alloys, has been tested by several authors [4-6,23]. According to Mondal et al.  there are some factors that may explain improvement on wear resistance such as: (1) the hard SiCp are protruded on the surface, and thus it will lead to a rougher surface; (2) the debris get accumulated around the SiCp.
So, by adding SiCp to the AlSi-2%wt.CNTs composite, it may lead to new advanced composite materials so-called hybrid metal matrix composites (HMMC) [16,24-26]. The increase in wear resistance in the case of hybrid composites was reported by several authors [16,25,26]. It has been proved that by adding graphite to an AlSi- SiCp  as a second reinforcement, the wear rates of the hybrid composite compared to SiCp reinforced composite decreased. As reported by Aruri et al.  the increase on wear resistance of both hybrid composites studied (Al-SiCp/Al2O3 and Al-SiCp/graphite) was attributed to the presence of both reinforcements. SiC particles acted like load bearing elements, while graphite acts like a solid lubricant. Also, Ames et al.  reported the improvement of wear behaviour when two reinforcements were added to an aluminium alloy (3 % graphite-20 % SiCp-A356). The higher wear rate was attributed also to the load bearing effect of SiC particles, but they reported that SiCp may also act as abrasives and can machine the counterface. This paper investigates the wear behaviour of an AlSi alloy reinforced by Multi-Wall Carbon Nanotubes (MWCNT) and SiC particles. The main purpose was to determine the combined effects (the advantages) of both constituent reinforcements (CNTs and SiCp) on wear behaviour in dry reciprocating sliding conditions. The purpose is to clarify if, when a certain reinforcement reached its optimal beneficial effect, another reinforcement could further increase the composite’s properties without compromising other relevant properties. 2. Experimental procedure 2.1. Fabrication of AlSi composites An AlSi alloy, powders size <325 mesh (<44µm), with chemical composition as listed in table 1, was used as matrix material. AlSi powder was purchased from AlfaAesar – Germany. Ni coated MWCNTs (outer diameter > 50 nm, length 0.5-2.0 µm, purity before coating>95wt% and ash <1.5wt%), and SiC particles (with 13 µm in size) were used as reinforcements. Ni coated MWCNTs were purchased from CheapTubes.com – USA. The AlSi-matrix composites were processed by the traditional hot isostatic pressing (HIP) technique. Applied pressure was 35x106 Pa for 10 minutes at 550ºC under vacuum (1 Pa). The mixing of the AlSi powders was done inside a closed stainless steel jar along with 12 steel milling balls (10 mm in diameter). The ball powder ratio is 10:1. The bottle rotated with constant speed (40 rpm) during 6 days (low-energy ball milling). Table 1 2.2. Microstructural and chemical characterization of AlSi composites The obtained AlSi composites and the worn surfaces (to observe the dominant wear mechanisms) were characterized by means of Scanning Electron Microscopy (SEM) / Energy Dispersive Spectrometry (EDS).
2.3. Hardness tests Vickers hardness tests were conducted according to standards, using a Shimadzu microhardness tester. Hardness measurements were conducted for all AlSi composites. Sixteen readings were taken for each condition from which the average value was calculated. The hardness tests were carried out with a load of 200 gf during 15 s. 2.4. Details of the reciprocating wear tests A reciprocating pin-on-plate tribometer PLINT-TE67/R was used to evaluate the wear characteristics of AlSi composites/GCI sliding pairs. Pins were machined from the unreinforced AlSi alloy and AlSi matrix composites (AlSi-2wt.%CNTs, AlSi-5wt.%SiCp and AlSi2wt.%CNTs-5wt.%SiCp). The dimensions of the pins are: radius of curvature 40 mm, thickness 3.5 mm and the arc length 20 mm. This AlSi composite can eventually be used for engine pistons or compression piston rings. The counterpart consisted of plates (40×18×5 mm) that were machined from grey cast iron (GCI) with a hardness of 338 HV. Table 2 presents the chemical composition of GCI. Table 2 Fig. 1 shows a schematic representation of the test performed in this work: applied normal load (Fn) on the pin and alternative displacement (d) of the GCI plate. Experiments were carried out with a normal load of 10 N and relative displacement amplitude of 10 mm, for a sliding distance of 148 m (for 2 hours), at a sliding speed of about 0.02 m/s. During the tests compressed air was flown to the contact zone in order to remove loose wear debris. The frequency of the reciprocating motion was 1 Hz for all tests. All wear tests were carried out under the same conditions. The only variable was the material of the pins (the reinforcement – CNTs, SiCp or CNTs-SiCp). An unreinforced AlSi alloy was used for comparison purposes. All tests were performed in environment temperature (20 ± 2°C). Fig. 1 The data acquisition system associated to the tribometer recorded different testing variables including coefficient of friction and sliding distance. Both pin and GCI plate were cleaned ultrasonically in alcohol before and after the tests and the amount of wear was measured by weight loss. The dominant wear mechanisms were characterized by SEM/EDS analysis.
3. Results and discussion 3.1. Microstructural characterization Microstructures of the unreinforced AlSi alloy and all AlSi matrix composites (after etching) are presented in fig. 2. SEM images revealed that CNTs, as expected are placed at the grain interfaces and also that there are some CNTs agglomerates (fig. 2b). In a previous work of the same authors  it has been shown that more than 93% of the agglomerates are less than 1 µm2 in area. The CNTs correspond to the white dots/areas. The average AlSi grain size is around 6 µm. Figure 2c shows the AlSi microstructure for 5wt.%SiCp, where can be seen the black SiC particles distributed in AlSi matrix. The SiC particles are visible at the grain interfaces as reported also by Balani et al.  and no interface was formed between SiC particles and AlSi matrix. Walczak et al.  reported that there can be formed interface between SiC particles and AlSi matrix, but if the processing route is other then HIP technique (e.g. squeeze casting route [27,29]). Fig. 2 Figure 2d shows the microstructure of the hybrid composite (Al-2wt.%CNTs-5wt.%SiCp). It can be observed the composite reinforcement (black SiC particles and the CNTs). There can be observed some CNTs agglomerates. The addition of SiCp seems that does not have any influence on the distribution of the CNTs. In both AlSi-5wt.%SiCp and Al-2wt.%CNTs-5wt.%SiCp composites can be observed that some SiC particles can form also clusters (fig. 2 c and d). These clusters can act like stress concentrations leading to microplasticity, as stated by other authors [30,31]. 3.2. Hardness values Fig. 3 shows the hardness results in the case of unreinforced AlSi alloy and of AlSi composites. As expected, the hardness increases with addition of the reinforcements (CNTs or SiCp). As compared to the unreinforced AlSi alloy, the AlSi-2%wt.CNT composite shows an increase on hardness of about 25%, as reported in another study of the same authors , while in the case of AlSi-5%wt.SiC composite of about 27%. The increase of hardness was higher in the case of hybrid composite, about 36%. The hardness results are in accordance with the other studies [32-34] and the main factor that governs the increase of hardness in both cases seems to be the volume fraction of the reinforcement. Fig. 3
The increase in hardness with the addition of the CNTs may eventually be explained based on the fact that the CNTs placed at the grain interfaces, create barriers to dislocations thus increasing strain hardening during plastic deformation, as reported by D.P. Mondal et al. . Regarding the increase in hardness of AlSi-5wt.%SiCp compared to unreinforced AlSi alloy is in accordance to other previous studies [32,35]. The increase in hardness was attributed to the high dislocation density in matrix induced by thermal mismatch between the matrix and the reinforcement  and to the harder reinforcements that impeded the movement of dislocations . In the case of the hybrid composites the hardness increased as compared to unreinforced AlSi alloy and to studied AlSi composites (fig. 3). These results are in accordance with the other studies [24,26,36]. The increase of hardness is due to strengthening effects of both reinforcements SiCp and CNTs (Shear lag , Thermal mismatch [25,27] and Orowan looping [38,39]). Due to different properties, shape and size of both reinforcements, it is expected that they have different contribution on the previously mentioned models. The behaviour of hybrid composites is a sum of inherent advantages and disadvantages of both reinforcements. Some other authors have been already proved the additional effect of the reinforcements on mechanical properties [24,27]. 3.3. Wear loss The volume losses of the AlSi pins (unreinforced AlSi alloy and AlSi - composites) and also of the mating GCI plates are shown in Fig. 4. When comparing all AlSi composites with the unreinforced AlSi alloy it can be clearly seen that the wear of all studied composites is less than that of unreinforced alloy. The wear volume decreased with the addition of CNTs or SiCp, and it further decreased with the incorporation of both reinforcements (CNTs and SiCp). Fig. 4 In the case of AlSi-2wt.%CNTs/GCI tribopair the volume loss decreased with about 8% for the AlSi-2wt.%CNTs composite (pin) and 29% for the GCI plate, as compared with the contact involving unreinforced AlSi alloy/GCI . As demonstrated by other studies [12-15,18,40], CNTs in the case of Al-matrix composite are an effective reinforcement for improving wear characteristics. The improvement in wear behaviour is explained in terms of CNTs dispersion in the matrix , CNTs agglomeration size and fraction , and on self lubricating effect of carbon content . In the case of AlSi-5wt.%SiCp/GCI tribopair the volume loss decreased about 6 % for the pin and 10% for the GCI plate, as compared with the contact involving unreinforced AlSi alloy/GCI. The improvement on wear behaviour when SiCp are incorporated into the AlSi alloy is in accordance with some other studies [4-6,23].
In the case of AlSi-2wt.%CNTs-5wt.%SiCp/GCI tribopair the volume loss decreased about 22% for the pin and 38% for the GCI plate, as compared with the contact involving unreinforced AlSi alloy/GCI. The combine effect of both reinforcements CNTs and SiCp in the AlSi matrix seem to have a beneficial role, once both pin and counterface material exhibited a reduction in wear volume, as compared to unreinforced AlSi/GCI tribopair and also to the AlSi composites/GCI tribopairs. Also in the present study the SiCp act like load bearing element and the CNTs have selflubrification effect. These effects will be later explained in the paper. Both reinforcements have a strengthening effect on the AlSi matrix, which also contributes to a better wear behaviour. It is worth to highlight that in the present work, by improving the wear resistance of all studied AlSi composites (pins), it was also improved the wear resistance of other part involved in the sliding contact (GCI plate). In practice it is desirable to achieve optimal operating condition of the system (as called tribosystem optimization). 3.4. Coefficient of friction Fig. 5 shows the evolution of the coefficient of friction (COF) with sliding distance in the case of AlSi-2wt.%CNTs-5wt.%SiCp hybrid composite against GCI. It is observed a typical evolution of the COF with the sliding distance for a reciprocating sliding wear test. After a first period corresponding to the running-in regime (where surfaces adapt to each other and COF changes significantly during the first period of sliding, increasing with the sliding distance) the COF enters in steady-state conditions and remains approximately constant during the whole test. Fig. 5 Fig. 6 presents the average COF for unreinforced AlSi alloy and of AlSi - composites. It can be seen that there is a slight decrease of COF values of the AlSi-composites as compared to unreinforced AlSi alloy. The COF values obtained in this study for AlSi – composites are approximately the same. Regarding the slight decrease of COF with the addition of CNTs, as reported in another study of the same authors , as the counterpart is a GCI and, consequently, there is a substantial amount of free carbon compared to the eventual contribution of carbon due to the CNTs content. The CNTs have two contributions on tribological behaviour of the composite: self lubrication effect and strengthening effect (increase the bonding between the grains on the Al matrix), so it is more difficult to remove them as confirmed by the mechanical properties results from another study of the same author . Due to their shape and size, mainly the CNTs that come from the agglomerates could roll between the mating surfaces . The agglomerates would have a higher effect on tribological properties if are released into the contact. There can be a disaggregation of these agglomerations due to the shear forces, leading to the appearance of individual CNTs that could roll into the sliding contact . Once the CNTs are released may behave as a third body that contributes to wear.
Fig. 6 The slight decrease of COF value observed in the case of AlSi alloy reinforced with SiCp as compared to unreinforced AlSi alloy can be explained based on the two mechanisms adhesion and abrasion. Related to adhesion there are two factors that may contribute to reduction of COF values: (i) the higher hardness of the matrix due to the presence of hard SiCp. Therefore, it is expected less adhesion between the pin composites and GCI plate. (ii) the presence of SiCp which work as load bearing elements [26,42] protect the matrix from wear. Regarding the second mechanism, abrasion, it is expected a higher COF values because the harder SiCp may penetrate the counter surface, as stated in . The presence of the SiCp also increases the hardness of the composite and is more difficult to cut down the picks of roughness, thus it is expected more abrasion of the SiCp and a harder matrix, as stated by Zhou et al. . Therefore, due to the combination of less adhesion and more abrasion, there is only a slight decrease on COF value. Later in this paper these mechanisms will be better explained based on the morphological analysis of both contact pairs. 3.5. Wear mechanism - SEM and EDS analysis GCI plates. Fig. 7 shows SEM images of the worn surfaces of GCI plates after sliding against unreinforced AlSi alloy and AlSi composites. Fig. 7 Fig. 8 shows a backscattered SEM images of GCI plates worn surface after sliding against AlSi-2wt.%CNTs-5wt.%SiCp hybrid composite and the EDS spectrum representative of the dark zones in the micrograph. Fig. 8 Regarding the worn surface morphology of GCI plates among the different materials used in this study, it can be seen from fig. 7 that even if the dominant wear mechanisms seems to be the same, such as: abrasion grooves (due to the reinforcement particles) and delamination marks, can be highlighted some differences. The GCI surface damage tends to decrease by the presence of CNTs or/and SiCp at mating surface, as revealed by the increased extension of smooth plateaus at GCI worn surface from Fig. 7 (a) to (d). In the case of the hybrid composite it can be observed (fig. 7d) that the groove size decreases in width indicating less plastic deformation (less abrasion) and also less delamination (less adhesion). These observations are in accordance with the volume wear loss between the plates used for sliding against unreinforced AlSi alloy and AlSi composites (fig. 4 – decreasing tendency of the volume loss of the GCI plates). The EDS analysis performed in the dark zones (Z1) presented in fig. 8 revealed some transfer of Al and Si derived from the pin counterface. EDS analysis in zone Z1 revealed the presence of the following elements: 19% O, 59% Al, 2% Si and 20% Fe. This oxygen content may indicate
the presence of some aluminum oxides. The transfer of Al and Si from the pin to the GCI plate means that the wear mechanisms of GCI also included adhesion. Besides Al, Si (coming from the matrix alloy) and O, there were found Fe and C (from the GCI). So, the main wear mechanism that governs the wear of the plates seems to be abrasion due to hard reinforcement particles and also adhesion as the AlSi matrix is softer then the GCI plate. AlSi composites (pins). Fig. 9 presents SEM images (130x magnification) of the worn surface of unreinforced AlSi alloy and of AlSi-composites pins (Fig.9 a1,b1,c1,d1) and also of the mating GCI pins (Fig.9 a2,b2,c2,d2). Fig. 9 Fig. 10 presents SEM images of the worn surface of AlSi-2wt.%CNTs-5wt.%SiCp hybrid composite with higher magnifications (1000x and 5000x). Fig. 11 shows the EDS analysis corresponding to distinct zones of the pin worn surface for the hybrid composite. It can be seen that zone Z1 shows the based material of pin, namely Al, Si and O. There is also Fe-rich and a small quantity of Mn transfer of material from the mating GCI plate. Fig. 10 Fig. 11 SEM images of the worn surfaces (Fig. 9 - magnification 130x) revealed that there is a clear difference in the worn surface topography of unreinforced AlSi alloy and AlSi composites (Fig.9 a1,b1,c1,d1). It can be clearly seen from the worn surface topography of the unreinforced AlSi alloy (fig. 9a1) is more uniform as compared to AlSi composite reinforced with CNTs (fig. 9b1). SEM images of the worn surface of AlSi-2wt.%CNTs pins (fig. 9b1) reveals that with the addition of the CNTs, on the pin contact surfaces can be observed two types of plateaus: a smooth plateaus and the other one with more voids, as reported in . More details regarding the worn surface topography of unreinforced AlSi alloy and AlSi-CNTs composite is given elsewhere . The strengthening mechanism of CNTs in AlSi sintered parts takes place (increasing the strength) [33,34,43,44] on the regions with well dispersed CNTs (on the smoother plateaus). Regarding the worn surface of AlSi-5%wt.SiCp composite (fig. 9c1), it can be observed that is very similar to the worn surface of unreinforced AlSi alloy (fig. 9a1). It can be observed a large plastic deformation, but it is lower as compared to unreinforced AlSi alloy and much lower than AlSi-2wt.%CNTs composite (fig. 9b1). In fig. 2c can be observed that there was formed a SiCp cluster that is considered a weakness point (lower bonding strength), so it is easier for the SiC particles to be pulled out. Generally, the pulled out particles may increase the abrasive wear of the composite due to the third body effect [5,25], but in our case they were taken off from the sliding area by the permanent air flow, so they will not have a significant effect on the wear behaviour of the AlSi composites based pins. This is in accordance with other studies  that
stated that the pull out mechanism increases the effect of abrasive wear, and consequently increased the wear loss. Regarding the worn surface of the AlSi-2wt.%CNTs-5 wt.%SiCp hybrid composite can be observed (fig. 9d1) similar plateaus as the ones observed in the case of unreinforced AlSi alloy: a smooth plateaus (adhesive wear) and the other one with more voids (abrasive wear). It seems that during sliding it is a competition between these two mechanisms, thus between abrasive and adhesive wear (fig. 9d1). It has been observed that the smoother region corresponds to the region where there is a good distribution of the CNTs and SiCp into the AlSi matrix. It can be seen that in the rougher regions (that seems to be less than the smoother ones) a layer of material has been removed as debris from the surface. The smother plateaus seems to be larger than in the case of AlSi-2wt.%CNTs composite, may be because the volume fraction is higher in the case of AlSi-2wt.%CNTs-5wt.%SiCp hybrid composite. It should be also mentioned that the amount of the trasnfered material is less in the case of AlSi-2wt.%CNTs-5wt.%SiCp hybrid composite from the pin to the plate (less dark zones in backscatter images –fig. 9d2) as compared to the unreinforced AlSi alloy and AlSi composites (Fig. 9a2,b2 and c2). It can be seen that no pull out mechanism can be observed in the case of hybrid composite (fig. 10). On fig. 10 can be observed a SiC particle that is debonded, and it is also fractured. It can be observed a lower level of plastic deformation in the case of AlSi hybrid composite as compared to the unreinforced AlSi alloy and AlSi composites.These happened simultaneously with the improvement on wear resistance (Fig. 4) of the AlSi - hybrid composite as compared to unreinforced AlSi alloy. Thus, it can be concluded that wear damage of unreinforced AlSi and AlSi composites based pins seems to be controlled essentially by two mechanisms: abrasive wear ( /pull-out of grains/particles) and adhesive wear that includes plastic deformation and material transfer between the mating surfaces. The AlSi hybrid composite seems to be controlled by the same mechanisms, but with wear that includes plastic deformation and material transfer between the mating surfaces. The introduction of both reinforcements (CNTs and SiCp) in the AlSi matrix seems to have a beneficial role, as AlSi-hybrid composite/GCI tribopair exhibited an improvement on wear resistance, as compared to unreinforced AlSi alloy/GCI and AlSi alloy- composites/GCI tribopairs. As referred above, the main contribution of the reinforcements are: (i) Strengthening effect of CNTs: A stronger bonding between AlSi grain interfaces due to the CNTs. This is basically in accordance with some of the proposed mechanisms, by George et al  namely thermal mismatch, Orowan looping and shear lag theory or also with Zang and coauthors  or even with Bustamante et al.  suggested mechanisms. Also, it should be mentioned that the CNTs agglomerations have detrimental effect on the strengthening, and they are responsible for voids nucleation.
(ii) Self-lubrication effect of CNTs. The CNTs and the CNTs agglomerates are released into the contact and there is a disintegration of these agglomerations due to the shear forces, leading to the appearance of individual CNTs that could roll into the sliding contact; (iii) Strengthening effect of SiCp: the strengthening of the matrix by SiC particles (SiCp increased the hardness of the composite); (iV) Load bearing elements: SiC particles act like load bearing elements (during sliding the SiC particles support the load and prevent the contact between the AlSi matrix and the GCI plate). Finally it should be emphasized that the approach based on two distinct reinforcements with different reinforcement mechanisms or the same reinforcement mechanism but acting at different scales (nano-scale or micro-scale) seems to be effective. As a fact the tensile strength with CNTs as reinforcement, presented its peak with 2% of CNTs, as shown in a previous paper . The same happened with the SiCp reinforcement that presented its saturation point, for tensile strength, at 5% of reinforcement. Thus, increasing the reinforcement content, in both cases, would allow to increase the wear behavior but it would substantially decrease the tensile strength. It was also reported that when the peak of tensile strength was achieved with one reinforcement (CNTs), it was possible to further increase the tensile strength by adding another type of reinforcement (SiCp). Thus it is concluded that the use of two reinforcements, by using two different reinforcement mechanisms or the same mechanism but at different scales, may provide better overall properties than by using one reinforcement alone. Thus, hybrid composites, as proposed in the present paper, provide better overall properties. CONCLUSIONS From the present investigation on the sliding wear behaviour of AlSi-composites/GCI tribopairs, the following conclusions can be drawn: - AlSi-2wt.%CNTs, AiSi-5wt.%SiCp and AiSi-2wt.%CNTs-5wt.%SiCp reinforced composites were successfully produced by hot-pressing technique. - Hardness of the all produced AlSi composites increased, and the hardness of the hybrid composite was higher as compared to unreinforced and also to the composites. Hardness of the hybrid composites increased due to the strengthening effect of both reinforcements CNTs and SiCp. - Both AlSi-2wt.%CNTs and AiSi-5wt.%SiCp composites experienced an improvement in the wear behaviour when compared to unreinforced AlSi alloy. The wear behaviour of AlSicomposites is controlled essentially by abrasive wear (with delamination/pull-out of grains/particles) and adhesive wear that includes plastic deformation and material transfer between the mating surfaces.
- The addition of both reinforcements (CNTs and SiCp) in AlSi matrix improved the wear behaviour of the AiSi-2wt.%CNTs-5wt.%SiCp hybrid composite when comparing to AlSicomposites. The wear behaviour of AlSi hybrid composite is controlled essentially by two mechanisms: abrasive wear and adhesive wear. - It is shown that by reinforcing AlSi alloy with both reinforcement the wear behaviour of tribopair (AlSi-hybrid composite/GCI) is improved, when compared with unreinforced AlSi /GCI and AlSi alloy- composites /GCI tribopairs, due to the strengthening effect of CNTs, selflubrication effect of CNTs and CNTs agglomerates, strengthening effect of SiCp and load bearing elements of SiC particles. ACKNOWLEDGEMENTS This work was supported by the Portuguese Foundation of Science and Technology through the project references PTDC/EME-PME/68664/2006, EXCL/EMS-TEC/0460/2012 and through the PhD grant with the reference SFRH/BD/44077/2008.
REFERENCES  S.V. Prasad, R. Asthana, Aluminum metal–matrix composites for automotive applications: tribological considerations, Tribol. Lett. 17 (2004), 445-453.  F.S. Silva, Fatigue on engine pistons – A compendium of case studies, Eng. Fail. Anal. 13 (2006) 480–492.  R.L. Deuis, C. Subramanian, J. M. Yellup, Dry sliding wear of aluminium composites-a review, Compos. Sci. Technol. 57 (1997) 415-435.  R.N. Rao, S.Das, D.P. Mondal, G. Dixit, Dry sliding wear behaviour of cast high strength aluminium alloy (Al–Zn–Mg) and hard particle composites, Wear 267 (2009) 1688–1695.  M. Walczak, D. Pieniak, M. Zwierzchowski, The tribological characteristics of SiC particle reinforced aluminium composites, ACME (2014), http://dx.doi.org/10.1016/j.acme.2014.05.003.  R.N. Rao, S. Das, Effect of matrix alloy and influence of SiC particle on the sliding wear characteristics of aluminium alloy composites, Mater. Des. 31 (2010) 1200–1207.  K. Umanath, S. T. Selvamani, Friction and wear behaviour of al6061alloy (SiCp +Al2O3p) hybrid composites, Int. j. innov. res. sci. eng. Technol. 3 (2011) 5441-5451.  K. Borodianskiy, A. Kossenko, M. Zinigrad, I mprovement of the Mechanical Properties of Al-Si Alloys by TiC Nanoparticles, Metall. Mater. Trans. A 44A,(2013) 4948—4953.  C. E. da Costa, L. de Aguiar, E.L. de Carvalho, V. A. Borras, Properties of AA6061 aluminum alloy reinforced with different intermetallics and ceramics particles, Proceedings of COBEM 2003, 17 International Congress of Mechanical Engineering Nov. 10-14 (2003) Sao Paulo.  M. O. Shabani, A. Mazahery, Prediction of wear properties in A356 matrix composite reinforced with B4C particulates, Synth. Met 161 (2011) 1226–1231.  A.P. Sannino, H.J. Rack, Dry sliding wear of discontinuously reinforced aluminum composites: review and discussion, Wear 189 (1995) 1-19.  S.R. Bakshi, A.K. Keshri, A. Agarwal, A comparison of mechanical and wear properties of plasma sprayed carbon nanotube reinforced aluminum composites at nano and macro scale, Mater. Sci. Eng. A 52 (2011) 3375–3384.  H.J. Choi, S.M. Lee, D.H. Bae, Wear characteristic of aluminium-based composites containing multi-walled carbon nanotubes, Wear 270 (2010) 12–18.  I.Y. Kim, J.H. Lee, G.S. Lee, S.H. Baik, Y.J. Kim, Y.Z. Lee, Friction and wear characteristics of the carbon nanotube–aluminium composites with different manufacturing conditions, Wear 267 (2009) 593–598.  S. Zhou, X. Zhang, Z. Ding, C. Min, G. Xu, W. Zhu, Fabrication and tribological properties of carbon nanotubes reinforced Al composites prepared by pressureless infiltration technique, Compos Part. A-Appl. S 38 (2007) 301–306.  W. Ames, A.T. Alpas, Wear Mechanisms in Hybrid Composites of Graphite-20 SiC in A356 Aluminum Alloy (AI-7 Pct Si-0.3 Pct Mg), Metall. Mater. Trans. A, 26A (1995) 85-98.  S.R. Bakshi, D. Lahiri, A. Agarwal, Carbon nanotube reinforced metal matrix composites – a review, Int. Mater. Rev. 55 (2010) 41-64.
 A.M. Al-Qutub, A. Khalil, N. Saheb, A.S. Hakeem, Wear and friction behaviour of Al6061 alloy reinforced with carbon nanotubes, Wear 297 (2013) 752–761.  L. Si, W. Chao, S. Lin, Y. Shuangchun, The research state of CNTs reinforced mental matrix composites, Int. J. of Adv. in Res. & Technol. 2 (2013) 243-245.  L. Peña-Parás, J. Taha-Tijerina, A. García, D. Maldonado, J. A. González, D. Molina, E. Palacios, P. Cantú, Anti-wear and extreme pressure properties of nanofluids for industrial applications”, Tribol. T. (2014) DOI: 10.1080/10402004.2014.933937.  O. Carvalho, G. Miranda, D. Soares, F. S. Silva, Carbon nanotube dispersion in aluminum matrix composites – quantification and influence on strength, Mech. Adv. Mat Struct. (2014), DOI: 10.1080/15376494.2014.929766.  O. Carvalho, M. Buciumeanu, D. Soares, J. Gomes, F. S. Silva, Improvement on sliding wear behaviour of Al/cast iron tribopair by CNT’s reinforcement of an Al alloy, Tribology Transactions (2014), DOI: 10.1080/10402004.2014.1002143.  D.P. Mondal, S. Das, R.N. Rao, M. Singh, Effect of SiC addition and running-in-wear on the sliding wear behaviour of Al–Zn–Mg aluminium alloy, Mater. Sci. Eng., A 402 (2005) 307– 319.  L. Poovazhagan, K. Kalaichelvan, A. Rajadurai, V. Senthilvelan, Characterization of Hybrid Silicon Carbide and Boron Carbide Nanoparticles-Reinforced Aluminum Alloy Composites, Procedia Eng. 64 (2013) 681 – 689.  S. Basavarajappa, G. Chandramohan, Dry Sliding Wear Behaviour of Hybrid Metal Matrix Composites, Mater. Sci. Medžig. 11, (2005) 253-257.  D. Aruri, K. Adepu, K. Adepu, K. Bazavada, Wear and mechanical properties of 6061-T6 aluminum alloy surface hybrid composites [(SiC + Gr) and (SiC + Al2O3)] fabricated by friction stir processing, J. Mater. Res.Technol. 2 (2013) 362–369.  D. S. Prasad, C. Shoba, Hybrid composites – a better choice for high wear resistant materials, J. Mater. Res.Technol. 3 (2014) 172-178.  X.N. Zhang, L. Geng, G.S. Wang, Fabrication of Al-based hybrid composites reinforced with SiC whiskers and SiC nanoparticles by squeeze casting, J. Mater. Process. Technol 176 (2006) 146–151.  B. Ralph, H.C. Yuen, W.B. Lee, The processing of metal matrix composites — an overview, J. Mater. Process. Technol. 63 (1997) 339-53.  G.P. Tandon, G.J. Weng, Stress Distribution in and Around Spheroidal Inclusions and Voids at Finite Concentration, J. Appl. Mech. 53 (1986) 511-518.  S.F. Corbin, D.S.Wilkinson, The influence of particle distribution on the mechanical response of a particulate metal matrix composite, Acta Metall. Mater. 42 (1994) 1311-1318.  A.A. Cerit, M.B. Karami, ù, F. Nair, K. Yildizli, Effect of Reinforcement Particle Size and Volume Fraction on Wear Behaviour of Metal Matrix Composites, Tribology in industry, Volume 30, No. 3&4, 2008.  D.P. Mondal, N.V. Ganesh, V.S. Muneshwar, S.Das, N. Ramakrishnan, Effect of SiC concentration and strain rate on the compressive deformation behaviour of 2014Al-SiCp composite, Mater. Sci. Eng. A 433 (2006) 18–31.  A. Mazahery, M. O. Shabani, Characterization of cast A356 alloy reinforced with nano SiC composites, Trans. Nonferrous Met. Soc. China 22 (2012) 275280.  G. E. Kiourtsidis, S. M. Skolianos, G. A. Litsardakis, Aging response of aluminium alloy 2024/silicon carbide particles (SiCp) composites, Mater. Sci. Eng. A 382 (2004) 351–361.
 D. S. Prasad, C. Shoba, N. Ramanaiah, Investigations on mechanical properties of aluminum hybrid composites, J. Mater. Res. Technol. 3 (2014) 79–85.  V.C. Nardone, K.M. Prewo, On the strength of discontinuous silicon carbide reinforced aluminum composites, Scripta. Metall. Mater. 20 (1986) 43-48.  R. George, K.T. Kashyap, R. Rahul, S. Yamdagni, Strengthening in carbon nanotube/aluminium (CNT/Al) composites, Scripta Mater. 53 (2005) 1159–1163.  Z. Zhang, D.L. Chen, Consideration of Orowan strengthening effect in particulatereinforced metal matrix nanocomposites: A model for predicting their yield strength, Scripta Mater. 54 (2006) 1321–1326.  K. Balani, A. Agarwal, Multiscale wear of plasma-sprayed carbon-nanotube-reinforced aluminum oxide nanocomposite coating, Acta Mater. 56 (2008) 5984–5994.  F. Dassenoy, L. Joly-Pottuz, J.M. Martin, T. Mieno, Carbon nanotubes as advanced lubricant additives, V.N. Popov and P. Lambin (eds.), Carbon Nanotubes, (2006) 237–238, Springer, Netherlands.  A.T. Alpas, J. Zhang, Effect of SiC particulate reinforcement on the dry sliding wear of aluminium-silicon alloys (A356), Wear 155 (1992), 83–104.  S.R. Bakshi, A. Agarwal, An analysis of the factors affecting strengthening in carbon nanotube reinforced aluminum composites, Carbon 49 (2011) 533– 544.  S.J. Yoo, S.H. Han, W.J. Kim, Strength and strain hardening of aluminum matrix composites with randomly dispersed nanometer-length fragmented carbon nanotubes,” Scripta Mater. 68 (2013) 711–714.  R. Pérez-Bustamante, C.D. Gómez-Esparza, I. Estrada-Guel, M. Miki-Yoshida, L. LiceaJiménez, S.A. Pérez-García, R. Martínez-Sánchez, Microstructures and tensile behaviour of carbon nanotube reinforced Cu matrix nanocomposites, Mater. Sci. Eng., A. 502 (2009) 159– 163.
Table 1 Chemical composition of AlSi alloy (wt.%) Al 87.3
Table 2 Chemical Composition of GCI Si P Cr Ni Cu S Mo Others 2.37 0.624 0.249 1.52 0.28 0.023 0.007 0.545
Composites reinforced by CNTs and SiCp were produced by hot-pressing technique.
The hardness of the hybrid composite was higher as compared to the composites.
The AlSi alloy reinforced by CNTs and SiCp showed superior wear behaviour.
The same mechanisms acting at different scales (nano/micro) are effective.
Fig. 1 Schematic test configuration: Fn – Normal applied load; d – alternated displacement amplitude
lomerates SiC particles
SiC clusters lomerates
Fig. 2 SEM images of the composites microstructures: a. unreinforced AlSi alloy; b. AlSi-2%wt.CNTs; c. AlSi-5wt.%SiCp and d. AlSi-2%wt.CNTs-5% wt.SiCp
100 80 60 40 20 0 AlSi
Materials Fig. 3 Hardness of the unreinforced AlSi alloy and all AlSi composites
Volume loss (mm3)
GCI plate pin
Materials Fig. 4 Variation on volume loss for unreinforced AlSi and AlSi - composites
0.8 0.6 0.4
0.2 0 0
50 100 Sliding distance (m)
Fig. 5 Evolution of COF with sliding distance of AlSi-2wt.%CNTs-5wt.%SiCp hybrid composite
Materials Fig. 6 Average COF of the unreinforced AlSi alloy and of the Al-Si composites
c d Fig. 7 SEM images of the worn surfaces of GCI plates after sliding against AlSi-based pins: a. unreinforced AlSi alloy; b. AlSi-2wt.%CNT; c. AlSi-5wt.%SiC and d. AlSi-2wt.%CNT5wt.%SiC
Fig. 8 Backscattered SEM image of GCI plate worn surface and EDS spectrum after sliding against (representative of the dark/grey zones in the micrograph) AlSi-2wt.%CNTs5wt.%SiCp hybrid composite
d1 d2 Fig. 9 SEM images of the worn surface of AlSi-based pins (130x magnification) and mating GCI plates (backscattered): a1/a2 - unreinforced AlSi alloy/GCI plate; b1/b2 - AlSi-2wt.%CNTs/GCI plate; c1/c2 - AlSi-5wt.%SiCp/GCI plate and d1/d2 AlSi-2wt.%CNTs-5wt.%SiCp/GCI plate
broken SiCp AlSi matrix
magnification 5000x magnification 1000´ Fig. 10 SEM images of the worn surface of AlSi-2wt.%CNTs-5wt.%SiCp hybrid composite
Fig. 11 SEM image (backscattered view) and EDS spectra (corresponding to Z1) of 2wt.%CNTs-5wt.%SiCp hybrid composite